Influence of the final temperature of investment healting on the tensile strength and Vickers hardness of CP Ti and Ti-6Al-4V alloy.
The aim of the work was to evaluate the influence of the temperature of investment healting on the tensile strength and Vickers hardness of CP Ti and Ti-6Al-4V alloy casting. Were obtained for the tensile strength test dumbbell rods that were invested in the Rematitan Plus investment and casting in the Discovery machine cast. Thirty specimens were obtained, fifteen to the CP Titanium and fifteen to the Ti-6Al-4V alloy, five samples to each an of the three temperatures of investment: 430 degrees C (control group), 480 degrees C and 530 degrees C. The tensile test was measured by means of a universal testing machine, MTS model 810, at a strain of 1.0 mm/min. After the tensile strength test the specimens were sectioned, embedded and polished to hardness measurements, using a Vickers tester, Micromet 2100. The means values to tensile tests to the temperatures 430 degrees C, 480 and 530: CP Ti (486.1 - 501.16 - 498.14 -mean 495.30 MPa) and Ti-6Al-4V alloy (961.33 - 958.26 - 1005.80 - mean 975.13 MPa) while for the Vickers hardness the values were (198.06, 197.85, 202.58 - mean 199.50) and (352.95, 339.36, 344.76 - mean 345.69), respectively. The values were submitted to Analysis of Variance (ANOVA) and Tukey Test that indicate differences significant only between the materials, but not between the temperature, for both the materials. It was concluded that increase of the temperature of investment its not chance the tensile strength and the Vickers hardness of the CP Titanium and Ti-6Al-4V alloy.
Oliveira
Pedro César Garcia
PC
Departament of Prosthodontics, Bauru School of Dentistry, University of São Paulo, Bauru, SP. pcdeoliveira@uol.com.br
Adabo
Gelson Luis
GL
Ribeiro
Ricardo Faria
RF
da Rocha
Sicknan Soares
SS
Avila
Fabiano Araújo
FA
do Valle
Accácio Lins
AL